Journal of Materials Science and Chemical Engineering, 2014, 2, 28-33
Published Online July 2014 in SciRes. http://www.scirp.org/journal/msce
How to cite this paper: Eziaku, O. (2014) Effect of an Organic Inhibitor on the Electrical Properties of High Carbon Steel in
Simulated Acid Environment. Journal of Materials Science and Chemical Engineering, 2, 28-33.
Effect of an Organic Inhibitor on the
Electrical Properties of High Carbon Steel
in Simulated Acid Environment
Department of Physics, University of Port Harcourt, Port Harcourt, Nigeria
Email: [email protected]
Received 9 April 2014; revised 8 May 2014; accepted 7 June 2014
Copyright © 2014 by author and Scientific Research Publishing Inc.
This work is licensed under the Creative Commons Attribution International License (CC BY).
The effect of 1-Phenyl-3-Methyl Pyrazol-5-one (HPMP) on the electrical properties of high carbon
steel in Hydrochloric acid (HCI), Trioxonitrate (v) acid (HNO3) and Perchloric acid (HCIO4) was
studied by weight loss method. The acidic medium caused a complete degradation of the electrical
properties of the coated and uncoated high carbon steel. However, the attack was more on the un-
coated coupons, which showed that HPHP is an effective corrosion inhibitor. HNO3 had the most
severe effect on the metal. The coupons coated with HPMP generally had higher values of resis-
tance (0.0155 Ω) and conductivity (6.20 mho/m) in HCI environment than the uncoated coupons
(0.0043 Ω) and (1.72 mho/m). Similar results were obtained for HNO3 and HCIO4 environments.
These values are lower than the values obtained for as-received coupons: −0.0466 and 8.64 mho/m
Electrical Properties, Corrosion, High Carbon Steel, 1-Phenyl-3-Methyl Pyrazol-5-One
Steel is one of the most important construction metals in the world. While this is common knowledge, many
people do not understand the difference between high carbon steel and other types of steel. High carbon steel is
any type of steel that contains over 0.8% of carbon but less than 2.11% of carbon in its composition. It has a
reputation for being especially hard, less formable and machinable, but the extra carbon makes it more brittle
than the other types of steel.
High carbon steel has many advantages over other options. It is excellent for making cutting tools such as
knives, saws, drill bits, farming and gardening equipment, compression springs, high ware applications, wood
cutting tools and high strength wire .
The failure of steel equipment due to acid corrosion in industries is widely reported, and the use of chemical
inhibitors for steel corrosion has been established to be the most practical and cost effective means of controlling
corrosion -. The extent of corrosion of metals among other factors depends on the nature of the material
used, the environment that the equipment is introduced to and the control measures used. Several Nitrogen and
Sulphur containing organic compounds have been used as corrosion inhibitors -. Corrosion inhibition is a
surface process which involves the specific adsorption of the organic compounds on the metal surface . The
adsorbed inhibitor then acts as a retardant to cathodic and anodic electrochemical process of the corrosion.
Electrical properties of metals are usually affected when corrosion occurs. Since corrosion affects the dimen-
sions or area of a material, one would infer that changes could occur in the electrical properties of the material
due to corrosion effect. This paper reports the effect of 1-Phenyl-3-Methyl Pyrazol-5-one (HPMP) on the elec-
trical properties of high carbon steel in various concentrations of HCI, HNO3 and HCIO4.
2. Materials and Methods
The high carbon steel strip was mechanically pressed cut into coupons of dimension 4.0 cm × 2.5 cm × 1.0 cm.
Each coupon polished and drilled at one end, was degreased in ethanol, dried in acetone and preserved in a de-
siccator. Solutions were prepared using analar reagents and distilled water. The HPMP Inhibitor was synthesized
as described by Vogel . The coupons were coated with the inhibitor by completely immersing them in a
mixture of ethanol and distilled water with 0.05M HPMP added to it. The coupons were retrieved after 1 hour,
blow dried and reweighed immediately to determine the mass of the film.
The three categories of coupons, namely: The as-received (control coupons, that were not exposed to the acid
medium), coated (coupons coated with HPMP inhibitor before exposure to the acid environment) and uncoated
(coupons that were exposed to the acidic medium without the HPMP inhibitor) coupons, were all subjected to
the current voltage measurement before and after the weight loss experiment.
3. Results and Discussion
The results from Table 1, show that HPMP inhibited High carbon steel in Hydrochloric acid and Nitric acid en-
vironments. The coated coupons had better corrosion resistance than the uncoated coupons. This is shown by the
lower values of weight loss recorded for the coated coupons. The coupons went into solution in Nitric acid at a
faster rate than in hydrochloric acid. This could be as a result of the nature of Nitric acid, as it is known to be a
strong oxidizing agent, and so it oxidizes the iron in high carbon steel at a faster rate.
However, it was observed that the coated coupons in perchloric acid environment had higher values of weight
loss than the uncoated coupons. This signifies that the inhibitor coating on the coupons was not stable and
therefore dissolved, thereby aiding the corrosion of the coupons in perchloric acid. This behavior is attributed to
Table 1. Weight loss (g) of coated and uncoated coupons in 0.8 M concentration of different acid environments.
Weight loss (g)
HCI HNO3 HCLO4
Uncoated coupon Coated coupon Uncoated coupon Coated coupon Uncoated coupon Coated coupon
1 1.3154 1.1484 0.6189 0.4594 1.0085 1.0003
2 1.5076 1.3224 0.7795 0.5847 1.0216 1.0262
3 1.5146 1.3557 1.0785 0.8338 1.0340 1.0460
4 1.5309 1.4266 1.2789 1.0353 1.0430 1.0920
5 1.5481 1.4697 1.5319 1.3353 1.0516 1.1482
6 1.5645 1.4890 1.6746 1.5202 1.0689 1.1847
7 1.5767 1.5098 1.8565 1.8009 1.0768 1.1963
the fact that perchloric acid is one of the strongest acids known . It is a powerful oxidizing agent and thus
causes fast dissolution of the coupons. It was also observed that the weight loss increased with increase in ex-
posure time for both uncoated and coated coupons.
Like all metals, steel can conduct electricity. The three main electrical properties of steel include its electrical
conductivity, electrical resistivity and temperature co-efficient. Electrical conductivity is the ability of a material
to conduct an electrical charge over a certain distance, while resistivity is the reciprocal of conductivity. The I-V
characteristics of high carbon steel in different concentrations of the acidic medium are shown on Figure 1. The
as-received coupon recorded higher current than those that were exposed to various concentrations of the acidic
medium. The acidic medium caused a complete degradation of the electrical properties of both the coated and
uncoated coupons, as shown in Table 2. There was a general decrease in the current flowing through the metal,
when compared with that of the as-received coupons. The coated coupons recorded higher current flow than the
uncoated coupons. The plots are shown on Figure 2.
Although there was a remarkable decrease in the I-V characteristics of the coupons exposed to the acid envi-
ronment, the normal Ohmic behavior, which is usually associated with metallic conductors still maintained. That
is, the exposed coupons were observed to exhibit the normal linearity variation pattern typical of electrical con-
ducting materials as shown in Figure 1. Similar results were obtained by Owate et al., Brikby et al., and Darry
and spear -.
Table 3 shows the resistance and conductivity of high carbon steel in various concentrations of the acids.
Both parameters were seen to decrease with increasing concentration. This result is in agreement with earlier
researchers  . Table 4 shows the resistance and conductivity of the coated and uncoated coupons in the
Figure 1. I-V Characteristics of uncoated high carbon steel in different con-
centrations of HCLO4.
Figure 2. I-V Characteristic of high carbon steel coupons in HCl, HNO3, HClO4.
Table 2. I-V characteristics of high carbon steel coupons in HCl, HNO3 and HCIO4.
HCl HNO3 HClO4
2 0.14 0.00 0.05 0.00 0.00 0.02 0.02
4 0.22 0.02 0.07 0.00 0.02 0.03 0.05
6 0.32 0.03 0.10 0.01 0.03 0.05 0.07
8 0.41 0.03 0.15 0.01 0.05 0.07 0.10
10 0.50 0.05 0.17 0.02 0.